Metal halide perovskites are attracting a lot of attention as next-generation light-emitting materials owing to their excellent emission properties, with narrow band emission1,2,3,4. However, perovskite light-emitting diodes (PeLEDs), irrespective of their material type (polycrystals or nanocrystals), have not realized high luminance, high efficiency and long lifetime simultaneously, as they are influenced by intrinsic limitations related to the trade-off of properties between charge transport and confinement in each type of perovskite material5,6,7,8. Here, we report an ultra-bright, efficient and stable PeLED made of core/shell perovskite nanocrystals with a size of approximately 10 nm, obtained using a simple in situ reaction of benzylphosphonic acid (BPA) additive with three-dimensional (3D) polycrystalline perovskite films, without separate synthesis processes. During the reaction, large 3D crystals are split into nanocrystals and the BPA surrounds the nanocrystals, achieving strong carrier confinement. The BPA shell passivates the undercoordinated lead atoms by forming covalent bonds, and thereby greatly reduces the trap density while maintaining good charge-transport properties for the 3D perovskites. We demonstrate simultaneously efficient, bright and stable PeLEDs that have a maximum brightness of approximately 470,000 cd m−2, maximum external quantum efficiency of 28.9% (average = 25.2 ± 1.6% over 40 devices), maximum current efficiency of 151 cd A−1 and half-lifetime of 520 h at 1,000 cd m−2 (estimated half-lifetime >30,000 h at 100 cd m−2). Our work sheds light on the possibility that PeLEDs can be commercialized in the future display industry.
This is a preview of subscription content, access via your institution
Subscribe to Nature+
Get immediate online access to Nature and 55 other Nature journal
Subscribe to Journal
Get full journal access for 1 year
only $3.90 per issue
All prices are NET prices.
VAT will be added later in the checkout.
Tax calculation will be finalised during checkout.
Get time limited or full article access on ReadCube.
All prices are NET prices.
The data that support the findings of this study are available from the corresponding authors upon reasonable request.
Kim, Y.-H. et al. Multicolored organic/inorganic hybrid perovskite light-emitting diodes. Adv. Mater. 27, 1248–1254 (2015).
Tan, Z.-K. et al. Bright light-emitting diodes based on organometal halide perovskite. Nat. Nanotechnol. 9, 687–692 (2014).
Cho, H. et al. Overcoming the electroluminescence efficiency limitations of perovskite light-emitting diodes. Science 350, 1222–1225 (2015).
Kim, Y.-H., Cho, H. & Lee, T.-W. Metal halide perovskite light emitters. Proc. Natl Acad. Sci. USA 113, 11694–11702 (2016).
Yang, X. et al. Efficient green light-emitting diodes based on quasi-two-dimensional composition and phase engineered perovskite with surface passivation. Nat. Commun. 9, 570 (2018).
Zhao, B. et al. High-efficiency perovskite–polymer bulk heterostructure light-emitting diodes. Nat. Photonics 12, 783–789 (2018).
Kim, Y.-H. et al. Comprehensive defect suppression in perovskite nanocrystals for high-efficiency light-emitting diodes. Nat. Photonics 15, 148–155 (2021).
Hassan, Y. et al. Ligand-engineered bandgap stability in mixed-halide perovskite LEDs. Nature 591, 72–77 (2021).
Xiao, Z. et al. Efficient perovskite light-emitting diodes featuring nanometre-sized crystallites. Nat. Photonics 11, 108–115 (2017).
Lin, K. et al. Perovskite light-emitting diodes with external quantum efficiency exceeding 20 per cent. Nature 562, 245–248 (2018).
Kim, Y.-H., Kim, J. S. & Lee, T. Strategies to improve luminescence efficiency of metal‐halide perovskites and light‐emitting diodes. Adv. Mater. 31, 1804595 (2019).
Park, M.-H. et al. Boosting efficiency in polycrystalline metal halide perovskite light-emitting diodes. ACS Energy Lett. 4, 1134–1149 (2019).
Cho, H., Kim, Y.-H., Wolf, C., Lee, H.-D. & Lee, T.-W. Improving the stability of metal halide perovskite materials and light-emitting diodes. Adv. Mater. 30, 1704587 (2018).
Liu, M., Matuhina, A., Zhang, H. & Vivo, P. Advances in the stability of halide perovskite nanocrystals. Materials 12, 3733 (2019).
Dong, Y. et al. Bipolar-shell resurfacing for blue LEDs based on strongly confined perovskite quantum dots. Nat. Nanotechnol. 15, 668–674 (2020).
Wehrenfennig, C., Eperon, G. E., Johnston, M. B., Snaith, H. J. & Herz, L. M. High charge carrier mobilities and lifetimes in organolead trihalide perovskites. Adv. Mater. 26, 1584–1589 (2014).
Herz, L. M. Charge-carrier mobilities in metal halide perovskites: fundamental mechanisms and limits. ACS Energy Lett. 2, 1539–1548 (2017).
Xu, W. et al. Rational molecular passivation for high-performance perovskite light-emitting diodes. Nat. Photonics 13, 418–424 (2019).
Meggiolaro, D., Mosconi, E. & De Angelis, F. Formation of surface defects dominates ion migration in lead-halide perovskites. ACS Energy Lett. 4, 779–785 (2019).
Zhang, L. et al. Suppressing ion migration enables stable perovskite light-emitting diodes with all-inorganic strategy. Adv. Funct. Mater. 30, 2001834 (2020).
Ahmed, G. H., Yin, J., Bakr, O. M. & Mohammed, O. F. Successes and challenges of core/shell lead halide perovskite nanocrystals. ACS Energy Lett. 6, 1340–1357 (2021).
Park, S. M., Abtahi, A., Boehm, A. M. & Graham, K. R. Surface ligands for methylammonium lead iodide films: surface coverage, energetics, and photovoltaic performance. ACS Energy Lett. 5, 799–806 (2020).
Wagstaffe, M. et al. An experimental investigation of the adsorption of a phosphonic acid on the anatase TiO2 (101) surface. J. Phys. Chem. C 120, 1693–1700 (2016).
Li, F., Zhong, H., Zhao, G., Wang, S. & Liu, G. Adsorption of α-hydroxyoctyl phosphonic acid to ilmenite/water interface and its application in flotation. Colloids Surfaces A Physicochem. Eng. Asp. 490, 67–73 (2016).
Xuan, T. et al. Highly stable CsPbBr3 quantum dots coated with alkyl phosphate for white light-emitting diodes. Nanoscale 9, 15286–15290 (2017).
Kim, H. et al. Proton-transfer-induced 3D/2D hybrid perovskites suppress ion migration and reduce luminance overshoot. Nat. Commun. 11, 3378 (2020).
Jeong, S.-H. et al. Characterizing the efficiency of perovskite solar cells and light-emitting diodes. Joule 4, 1206–1235 (2020).
Pazos-Outon, L. M. et al. Photon recycling in lead iodide perovskite solar cells. Science 351, 1430–1433 (2016).
Stranks, S. D., Hoye, R. L. Z., Di, D., Friend, R. H. & Deschler, F. The physics of light emission in halide perovskite devices. Adv. Mater. 31, 1803336 (2019).
Cho, C. et al. The role of photon recycling in perovskite light-emitting diodes. Nat. Commun. 11, 611 (2020).
Cho, C. & Greenham, N. C. Computational study of dipole radiation in re‐absorbing perovskite semiconductors for optoelectronics. Adv. Sci. 8, 2003559 (2021).
Song, J. et al. Over 30% external quantum efficiency light‐emitting diodes by engineering quantum dot‐assisted energy level match for hole transport layer. Adv. Funct. Mater. 29, 1808377 (2019).
Kim, Y.-H. et al. Exploiting the full advantages of colloidal perovskite nanocrystals for large-area efficient light-emitting diodes. Nat. Nanotechnol. 17, 590–597 (2022).
Dai, X. et al. Solution-processed, high-performance light-emitting diodes based on quantum dots. Nature 515, 96–99 (2014).
Woo, S.-J., Kim, J. S. & Lee, T.-W. Characterization of stability and challenges to improve lifetime in perovskite LEDs. Nat. Photonics 15, 630–634 (2021).
Cho, H. et al. High-efficiency polycrystalline perovskite light-emitting diodes based on mixed cations. ACS Nano 12, 2883–2892 (2018).
Palik, E. D. & Ghosh, G. Handbook of Optical Constants of Solids (Academic Press, 1998).
This work was supported by the National Research Foundation of Korea (NRF) grant funded by the Korea government (Ministry of Science, ICT and Future Planning) (NRF-2016R1A3B1908431). G.-S.P was supported by the DGIST R&D Program (22-CoE-NT-02) by the Korea government (Ministry of Education and Ministry of Science, ICT and Future Planning).
The authors declare no competing interests.
Peer review information
Peer review information
Nature thanks Lina Quan, Zhanhua Wei and the other, anonymous, reviewer(s) for their contribution to the peer review of this work.
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Extended data figures and tables
SEM images of perovskite thin films made of 1.2M precursor solution with a, 0% (3D), b, 2.5%, c, 5%, d, 10% (in situ particle) molar ratio of BPA molecule relative to PbBr2. e, HAADF-STEM image and EDS elemental maps of P (green), Br (yellow), and Pb (red), respectively. f, HAADF-STEM image and EDS elemental maps of a single perovskite grain showing the uniform dispersion of P (green), Br (yellow), and Pb (red) on the grain.
Extended Data Fig. 2 Morphological characterization during in situ core/shell particle synthesis process.
a, SEM image of a perovskite thin film (after 1s of reaction time with BPA-THF solution) showing small grains cracked out from large 3D grain. b, STEM image of 50 nm-size perovskite crystal during in situ core/shell synthesis process. Yellow arrows indicate the defective perovskite surfaces that can be bound with BPA. c, HR-TEM image of another perovskite crystal showing ultra-small nanocrystals segregated during in situ core/shell synthesis process. Insets: Magnified HR-TEM images of ultra-small nanocrystals taken from the white-boxed regions labelled C1 and C2. d, e, High-resolution HAADF-STEM images of single perovskite nanograins with decreasing grain size. Magnified HAADF-STEM images of the grain surfaces (D1, D2, E1, E2, F1, F2, G1, G2) demonstrate that the BPA shell coverages on the grain surfaces gradually increase and the defective surface regions decrease as the grain size decreases.
a, High-resolution HAADF-STEM image of single perovskite grain formed during in situ core/shell synthesis process. b, c, Atomic-scale HAADF-STEM (b) and ABF-STEM (c) images of the boxed area denoted in a. d,e, Magnified HAADF-STEM (d) and ABF-STEM (e) images of the boxed area shown in b and c to indicate the positions of EELS acquisition. f, EEL spectra acquired at the atomic positions labelled A, B, and C in d, e. g, EEL spectrum in the energy-loss range of the N-K and O-K edges acquired at the position labelled C. The O-K peak indicates the presence of BPA shells, but N-K peak is simply a background signal from the silicon nitride TEM window grid.
Extended Data Fig. 4 SEM image of low-concentration (0.6 M) perovskite thin films with different reaction time between BPA solution and perovskite thin film.
a, 3D perovskites without reaction, b, 1 s, c, 15 s, d, 30 s of exposure time to BPA-THF solution before spin-drying. Coloured regions indicate initial large crystals (red) and split nanograins (green). e, Schematic illustration of the growth process of BPA macroparticle domain and perovskite crystal forming in situ core/shell structure.
a, TEM image and b, c, magnified HAADF-STEM images of in situ core/shell perovskite thin films. d, HAADF-STEM image of in situ core/shell grains and EDS elemental maps of P (red), Pb (yellow), and Br (green), respectively. The EDS maps clearly show the uniform dispersion of P (red) over macrograins. e, HAADF-STEM image of single macrograins consists of in situ core/shell nanoparticles. f, EDS spectrum acquired at the location of the red circled region in e.
a, PL spectra and b, normalized PL spectra of quartz/perovskite thin film measured in integrating sphere. c, External PLQE versus internal radiation efficiency (ηrad) (i.e. internal quantum efficiency, IQE) of perovskite film calculated considering the influence of perovskite reabsorption30,31. The external PLQE of the in situ core/shell structure was 46%, which corresponds to an IQE of 88%. d–i, Temperature-dependent PL spectrum and corresponding integrated PL intensity with calculated activation energy for: d,g, 3D, e,h, in situ particle, f,i, in situ core-shell perovskite thin films.
a, Current density versus voltage; b, luminance versus current density; c, normalized EL spectra; d, CIE coordinate of in situ core/shell PeLEDs; e, power efficiency versus luminance; f, current efficiency versus luminance of PeLEDs based on 3D, in situ particle, in situ core/shell structure. g, Angle-dependent EL intensity and h, luminance histogram of PeLEDs based on in situ core/shell structure. i, EQE histogram of the PeLEDs based on in situ core/shell structure with different processing condition. As the temperature of the glove box increases or the A-NCP process is delayed, the grain size of the spin-coated perovskite thin film increases, which slows the penetration of the BPA solution into perovskite crystal and prevents full conversion of them into the in situ core/shell structure.
a, Luminance versus voltage; b, EQE versus current density of large-area devices based on in situ core/shell perovskites. c–f, Photographs of large-area devices (pixel size: 120 mm2) operating at: c, < 10 cd m−2; d, 1,000 cd m−2; e, 100,000 cd m−2; and f, 100,000 cd m−2 under daylight, showing uniform emission over the pixel.
a, Luminance versus time of PeLEDs based on 3D, in situ particle, and in situ core/shell perovskites at initial brightness of 10,000 cd m−2, and b, corresponding driving voltage versus operation time.
About this article
Cite this article
Kim, J.S., Heo, JM., Park, GS. et al. Ultra-bright, efficient and stable perovskite light-emitting diodes. Nature 611, 688–694 (2022). https://doi.org/10.1038/s41586-022-05304-w